Oxygen vacancies in transition metal and rare earth oxides: Current state of understanding and remaining challenges
Oxygen vacancies in transition metal and rare earth oxides: Current state of understanding and remaining challenges
Surface Science Reports 62 (2007) 219–270 www.elsevier.com/locate/surfrep Oxygen vacancies in transition metal and rare earth oxides: Current state of understanding and remaining challenges M. Verónica Ganduglia-Pirovano∗, Alexander Hofmann, Joachim Sauer Humboldt-Universität zu Berlin, Institut für Chemie, Unter den Linden 6, D-10099 Berlin, Germany Accepted 26 March 2007 Abstract Defects at transition metal (TM) and rare earth (RE) oxide surfaces, neutral oxygen vacancies in particular, play a major role in a variety of technological applications. This is the motivation of numerous studies of partially reduced oxide surfaces.
We review, discuss, and compare theoretical data for structural and electronic properties and energetic quantities related to the formation of oxygen defects at TM and RE oxide surfaces using TiO2, ZrO2, V2O5, and CeO2 as examples. Bulk defects, as far as relevant for comparison with the properties of reduced surfaces, are briefly reviewed. Special attention is given to the fate of the electrons left in the system upon vacancy formation and the ability of state-of-the- art quantum-mechanical methods to provide reliable energies and an accurate description of the electronic structure of the partially reduced oxide systems.
c 2007 Elsevier B.V. All rights reserved. Contents 1. Introduction . . 220 2. Models and methods . . 221 3. Titanium oxide . . 222 3.1. TiO2 applications and basic information . . 222 3.2. Experimental findings on oxygen vacancies . . 222 3.3. Reduced TiO2 rutile (110) surface . . 224 3.3.1. Structure relaxation and electronic structure . . 224 3.3.2. The rutile TiO2(110) surface defect formation energy . . 229 3.4. Reduced TiO2 anatase surfaces . . 233 3.5. Reduced rutile and anatase TiO2 bulk . . 235 3.6. Summary TiO2 . . 237 4. Zirconium oxide . . 237 4.1. ZrO2 applications and basic information .
. 237 4.2. Experimental findings on oxygen vacancies . . 238 4.3. Reduced ZrO2 bulk phases . . 238 4.3.1. Structure relaxation and electronic structure . . 239 4.3.2. The ZrO2 bulk defect formation energy . . 242 4.4. Reduced t-ZrO2 surfaces . . 243 4.5. Summary ZrO2 . . 243 5. Vanadium oxide . . 243 ∗ Corresponding author. E-mail address: firstname.lastname@example.org (M.V. Ganduglia-Pirovano). 0167-5729/$ - see front matter c 2007 Elsevier B.V. All rights reserved. doi:10.1016/j.surfrep.2007.03.002
220 M.V. Ganduglia-Pirovano et al. / Surface Science Reports 62 (2007) 219–270 5.1. Applications and basic information . . 243 5.2. Experimental findings on oxygen vacancies . . 244 5.3. Reduced V2O5(001) surface . . 245 5.3.1. Structure relaxation and electronic structure . . 245 5.3.2. The V2O5(001) surface defect formation energy . . 248 5.4. Summary V2O5 . . 250 6. Cerium oxide . . 250 6.1. CeO2 applications and basic information . . 250 6.2. Experimental findings on oxygen vacancies . . 251 6.3. Reduced low-index CeO2 surfaces . . 252 6.3.1. Structure relaxation and electronic structure .
. 252 6.3.2. The surface defect formation energy . . 256 6.4. Reduced CeO2 bulk . . 257 6.5. Summary CeO2 . . 260 7. Similarities and differences between TiO2, ZrO2, V2O5, and CeO2 . . 260 8. Summary and outlook . . 263 Acknowledgements . . 264 References . . 264 1. Introduction Transition metal (TM) oxides constitute an important class of inorganic solids exhibiting a very wide variety of structures and electronic and magnetic properties that are due to the nature of the outer d states [1,2]. They are of great importance for a number of a technological applications such as heterogeneous catalysis, corrosion-protective coating of metals and microelectronic devices.
Point defects in TM oxides such as vacancies and interstitials account for the transport properties of ionic solids. Furthermore, bulk defects play a significant role in determining surface properties where, for example, annealing to high temperatures is necessary. In addition, an important issue in TM oxide-based heterogeneous catalysis is the role of surface defects in determining the activity and selectivity of the catalyst. The existence of reduced surface centers — and hence the presence of neutral oxygen vacancies — is sometimes necessary for any activity. Ultimately, the potential of TM oxides in applications is related to the ability of the metal atoms to assume multiple oxidation states — for instance, vanadium can have the oxidation states II, III, IV, and V.
This characteristic is not exclusive to transition (d) metal oxides and a representative example is given by ceria-based materials . Many of the key properties of ceria, a rare earth (RE) oxide, arise from the fact that cerium has two stable oxidation states, namely, III and IV, in which f electron states are partially occupied or empty, respectively.
Oxygen vacancies at (TM and RE) oxide surfaces (or in the bulk) alter the geometric and electronic structure as well as chemical properties of the host system. In turn, the host system will largely determine the properties of the vacancies. The expectation that a fundamental understanding (i.e., microscopic) of these defects will help to elucidate the effect that they have on the system’s functionality has been the driving force for pursuing experimental and theoretical research on reduced materials. For years oxygen vacancies have been detected and investigated using a variety of spectroscopic techniques, however, much has been learned recently about the structure of defective surfaces using scanning probe techniques.
In spite of that, there are still difficulties in the experimental determination of the vacancy-induced lattice relaxations, and information about the vacancy formation energy (hence defect stability) is not always experimentally obtainable. Therefore, a great number of theoretical studies on oxygen removal from TM and RE oxides have appeared in the literature. In particular, isolated oxygen vacancies at differently oriented surfaces and in the bulk have received much attention. Strong interactions can occur between defects, causing them to cluster or order. Yet, isolated defects (or a low concentration of them) have been the natural starting point for the theoretical studies.
In this article, we consider the formation of oxygen vacancies at TM and RE oxide surfaces using TiO2, ZrO2, V2O5, and CeO2 as examples. The partially reduced bulk oxides are also considered. The interest on these particular oxide surfaces is their importance for heterogeneous catalysis and other industrial applications. Their specific applications that are the deeper motivation for most of the performed work will be briefly mentioned in each of the sections that cover basic properties of the oxides. The focus is on theoretical studies and the more recent literature (after 1990). Inclusion of experimental studies would render a review unmanageably large given the vast number of experimental studies published since 1990 on oxygen defects for the systems considered.
Nevertheless, the key experimental findings on the properties of the reduced systems are mentioned. One question of fundamental interest is: What is the electronic structure of the reduced oxides systems? In other words, when neutral oxygen atoms are removed, which states do the electrons left in the system populate? Another question, which is perhaps more practical, is: What is the energy required to form the oxygen defects? Answering these questions has provided a very strong motive to investigate the nature of neutral oxygen defects in the specific chosen systems at the atomistic level using density functional theory (DFT); see, e.g., Refs.
[4–29] (TiO2), Refs. [29–35] (ZrO2), Refs. [36–42] (V2O5), and Refs. [43–
M.V. Ganduglia-Pirovano et al. / Surface Science Reports 62 (2007) 219–270 221 54] (CeO2). Different exchange–correlation functionals have been applied, including the local density approximation (LDA) and generalized gradient approximation (GGA) for exchange and correlation [55–57], as well as hybrid functionals such as Becke–Lee–Yang–Parr (B3LYP), which contain a portion of exact exchange (20%) [58,59]. The Hartree–Fock (HF) and DFT+U approaches [60–63] have also been used. Defects have been modelled using either (embedded) cluster or the supercell approach, i.e., applying periodic boundary conditions.
While several theoretical articles and reviews that compare defective wide-gap oxides such as SiO2, MgO, SnO2, α-Al2O3, and HfO2 (i.e., non-TM oxides in particular) were written in recent years [64–71], a comprehensive review of theoretical insights into oxygen vacancy properties in TM and RE oxides in general and in those considered in this report in particular, is lacking. In this report, an attempt is made to critically review the ability of different computational methods to provide reliable (geometrical and electronic) structures and energies for oxygen defects for selected examples of TM and RE oxides.
The four oxides, TiO2, ZrO2, V2O5, and CeO2 are discussed in Sections 3, 4, 5 and 6, respectively. Each section starts with the basic structural and electronic properties of the bulk and selected low-index surfaces. Then the important experimental findings on the reduced systems are summarized. In the following subsections the theoretical insights into the structural and electronic properties and energetic quantities related to the formation of surface oxygen defects and in the bulk are reviewed and discussed. The article ends with a comparison of the systems considered and an outlook of the remaining challenges for first-principles studies in the field of oxygen defects in oxide materials.
2. Models and methods In the so-called periodic approach to study solids, bulk and surfaces, the Schrödinger equation is (approximately) solved for the atoms of a unit cell containing a given number of atoms, subject to periodic boundary conditions in three dimensions. Surfaces are modelled in a supercell approach. Here one considers the periodic repetition of a two-dimensional periodic slab of the crystal together with a sufficiently thick vacuum layer, in the direction parallel to the surface normal. Hence, in the periodic approach one models two surfaces, one at each side of the slab. The thickness of the slab and vacuum layer are chosen so that the mutual interaction between the two surfaces of a slab and between those of periodic images, respectively, vanish.
The presence of a point defect in the surface unit cell (typically on one side of the slab) results in its periodic repetition and a high concentration of surface defects. Increasing the size of the unit cell in the surface plane reduces the defect concentration, but increases the computational cost. Similar considerations apply to defects in the bulk unit cell, repeating in three directions. We recognize that the defect concentrations accessible to computer simulations are typically much higher than those encountered in experiments. An alternative approach is the use of cluster models. Here only a finite number of atoms are explicitly considered to describe a part of a solid system whereas the rest of the crystal is treated by embedding techniques.
There is an important advantage in the use of clusters in describing point defects — an infinite dilution is considered. Ideally there should be no dependence of the calculated properties on the embedding, size, and shape of the cluster used, thus careful checks have to be performed.
Density functional theory has become a widely used tool for calculations of the properties of solids and molecules, employing both periodic and cluster approaches. Standard implementations of DFT are based on the Kohn–Sham equations and use LDA or GGA for the exchange–correlation functional. Three GGA functionals, namely PW91 , PBE , and RPBE , have been used in studies of oxygen defects in the TM and RE oxide systems considered in this review. A number of failures are known to exist in LDA and all currently used GGA functionals, for example the underestimation of band gaps, the gross overestimation of electron delocalization and metallic character, the overestimation of atomization energies of molecules and solids, and the underestimation of energy barriers for molecular reactions.
These problems are a consequence of employing approximations to the unknown exchange–correlation functional. Another source of error is the lack of exact cancellation of the Coulombic self-interaction, which stabilizes solutions with delocalization of spin density and, as a result, the electronic structure of highly localized magnetic systems is not correctly reproduced. For these reasons, the description of oxygen defects on TM and RE oxide surfaces and in the bulk employing standard DFT is expected to show deficiencies. These will particularly relate to the electronic properties of the reduced systems, specifically, the location of the electrons left in the system upon reduction, the population of specific electronic states by these electrons, resulting in occupied states in the band gap, and the actual position of these (defect) states within the gap.
Shortcomings are also anticipated in the defect formation energy. In this report we illustrate the merits and limits of local and gradient- corrected functionals as applied to reduced TiO2, ZrO2, V2O5, and CeO2 bulk and surfaces.
The above-mentioned inadequacies of GGA functionals can be partly removed by admixture of a fixed amount of Fock exchange to the exchange–correlation functional. These hybrid functionals give significant improvement over GGA for many molecular properties and are very popular in molecular quantum chemistry. Possibly the most widely used hybrid functional is B3LYP [58,59]. Despite the important impact of hybrid functionals on molecular quantum chemistry, their applications to periodic solids used to be linked to Gaussian basis sets (see, e.g., Refs. [23,25,72–77]). Due to progress in plane-wave based algorithms [78,79] and computer speed, hybrid functionals such as HSE03 [80–82] and PBE0 [83– 85] have been implemented recently in widely used plane- wave basis set codes [86–89].
The hybrid (periodic and cluster) approach has been successfully applied to selected defective TM oxide surfaces [12,23,25,40]. Compared to GGA functionals, an improved description of the electronic
222 M.V. Ganduglia-Pirovano et al. / Surface Science Reports 62 (2007) 219–270 structure and more accurate energies have been obtained. The use of cluster models, in particular, allows for the explicit inclusion of correlation effects employing approaches such the Møller–Plesset perturbation theory. The application of such approaches to the electronic structure of point defects at TM or RE oxide surfaces is, however, still rare . A number of more pragmatic approaches have been developed to address the deep seated problems of local and gradient-corrected functionals such as the self-interaction correction (SIC)  and the DFT + U approach.
This latter method was originally proposed by Anisimov and co-workers [60–63] to account for correlations resulting from strong on- site Coulomb and exchange interactions, as an extension of the LDA approach based on the lessons learned from Hubbard model studies [92–94]. In practice, in these DFT(LDA/GGA)+ U approaches one identifies a set of atomic-like orbitals that are treated with an orbital-dependent potential and an associated screened on-site Coulomb and exchange interaction parameter, U and J, respectively . The method, although initially tied to the linear muffin-tin orbital (LMTO) approach, has been reformulated for different basis sets [96–99].
The DFT + U approach has been applied recently to partially reduced RE systems [48–54]. Yet, questions regarding the proper way of specifying the atomic-like orbitals, and of deriving the best value for the so-called effective Hubbard-U parameter (U0 = U − J) are still under debate.
Last, but not least, generation of the (norm-conserving or ultra-soft) pseudopotentials used in periodic plane-wave calculations (see Refs. [100,101] and references therein) still is a tricky, cumbersome, and error-prone task. Ill-behaved pseudopotentials may affect the description of defective systems, the electronic structure in particular. Yet, deficient pseudopotentials are easily spotted if results are compared to those obtained using all-electron methods. Examples of this and the above-mentioned aspects of calculations on reduced TM and RE oxides systems using different models and methods will be discussed in more detail in following sections.
The average oxygen defect formation energy EO f is defined as EO f = 1/Ndef[Edef − Efree + EO], (1) where Edef, Efree, and EO represent the total energies of the reduced and defect-free system, and the free oxygen atom, respectively. Ndef is the number of oxygen defects in the model. In the following, E 1 2 O2 f indicates the use of the molecular reference energy in Eq. (1), i.e., E 1 2 O2 f = 1/Ndef Edef − Efree + 1 2 EO2 . (2) A positive value for E 1 2 O2 f indicates that the vacancy formation is endoenergetic and the difference between EO f and E 1 2 O2 f is just half the dissociation energy of the O2 molecule (E 1 2 O2 d ).
3. Titanium oxide 3.1. TiO2 applications and basic information Titanium dioxide is the model system in the surface science of TM oxides . It is by far the most extensively studied TM oxide system (see Ref.  and references therein). Well ordered, nearly perfect surfaces can be produced relatively easily; it is used as a support of both metal and oxide catalysts, as a photocatalyst, as a gas sensor, as a corrosion-protective coating, and in electric devices such as varistors. Titanium dioxide crystallizes into three main phases, rutile, anatase, and brookite. However, only rutile and anatase play any role in the applications of TiO2.
In both structures, the basic building block consists of Ti atoms surrounded by six oxygen atoms in a more or less distorted octahedral configuration (see Fig. 1). The bulk unit cell compositions are Ti2O4 and Ti4O8, respectively. In all three structures, the stacking of the octahedra results in threefold coordinated oxygen atoms. Rutile is the most abundant polymorph in nature. Most crystal growth techniques yield TiO2 in the rutile phase, thus this phase has been studied extensively. Relative to rutile there are fewer investigations of the anatase phase, although it constitutes most of the commercially produced material.
In the following, if the phase is not explicitly mentioned, rutile is meant. Both rutile and anatase are insulators with band gaps of 3.0 and 3.2 eV, respectively . Anatase is less dense and less stable than rutile at ambient pressures and temperatures (see Ref.  and references therein). The transition temperature depends on a variety of factors including impurities, sample history and crystal size. Indeed, nanocrystalline TiO2 may be phase selected by controlling the particle size, as well as other experimental conditions such as temperature . The oxygen terminated (110) and (101) oriented (1 × 1) surfaces are the most stable rutile and anatase surfaces, respectively [102,106–108].
Both surfaces have sixfold and fivefold coordinated Ti atoms (Ti(6) and Ti(5)), as well as threefold and twofold coordinated O atoms (O(3), O(2), respectively, see Fig. 2). The removal of the latter, so-called bridging oxygen atoms is a subject of much interest and debate. 3.2. Experimental findings on oxygen vacancies The titanium–oxygen phase diagram is very rich with a variety of crystal structures . When point defects (predominantly oxygen vacancies) are created in the bulk or at surfaces, they cause important changes in the electronic structure that affect the performance of the material in various applications.
Consequently, the properties of reduced TiO2 have been the subject of considerable experimental and theoretical interests [7–19,22,23,25–29]. The sheer number of experimental investigations, in particular, excludes a comprehensive listing, and we refer the reader to the recent review by Diebold .
The defect structure of TiO2−x is a complex issue because a family of stable Magnéli phases [110,111] is found to occur between Ti2O3 and TiO2. At low concentrations (x < 10−4) the
M.V. Ganduglia-Pirovano et al. / Surface Science Reports 62 (2007) 219–270 223 Fig. 1. Bulk structures of rutile (left) and anatase (right) TiO2 phases. Fig. 2. The bulk truncated (110) and (101) surfaces of rutile (left) and anatase (right), respectively. Shown are four- and three-layer (1 × 1) slabs, respectively. The dotted lines indicate the repeating unit (one-layer) in the direction perpendicular to the surface.
oxygen vacancies are accommodated as point defects while for higher degrees of reduction crystallographic shear (CS) planes are formed, and the point defects eliminated. It is beyond the scope of this work to discuss the formation of CS planes and the most stable structure for a given stoichiometry. Heating TiO2 bulk single crystals in vacuum leads to deviations from the 1:2 stoichiometry as firstly reported by Gray et al. , and is accompanied by visible color changes from transparent to light and, in turn, dark blue . These deviations were later attributed to conduction electrons trapped at Ti sites forming (electron paramagnetic resonance) EPR- active TiIII species .
The EPR studies revealed that darker rutile crystals exhibit higher concentrations of TiIII centers associated to bulk defects such as crystallographic shear planes , that may extend all the way to the surface . The characteristic EPR signals attributed to TiIII ions were also observed after excitation of anatase TiO2 samples with UV light , but the signal may disappear at increasing temperature if the particles are small . Reduced TiO2 crystals exhibit n-type doping, and are widely used in photocatalysis (see Ref.  and references therein).
There is overwhelming spectroscopic and chemical evidence for the presence of oxygen defects on (rutile and anatase) samples sputtered and annealed in UHV. These are attributed to bridging oxygen vacancies. Their concentration is reported as several per cent [119,120]. Anatase surfaces show, however, less tendency to release lattice oxygen atoms. For the (110) rutile surface, in particular, scanning tunneling microscopy (STM) has uncovered a large amount of information about oxygen defects in the bridging oxygen  oriented rows that includes their diffusion and adsorption on the defective surface [102,121–125].
The latter topic has blossomed after Haruta’s discovery  that nanosized TiO2 supported gold clusters exhibit unique catalytic properties [127–129]. It is assumed that the presence of defects on the substrate plays an important role in the catalytic activity (see additional references in the recent survey by Diebold ), but experimental evidence has not yet been provided.
Regardless of the location of the oxygen vacancy (i.e., in the bulk or at a surface) the presence of TiIII ions in the reduced systems has been reported. In the following, we summarize the key features of the experimental evidence for their existence
224 M.V. Ganduglia-Pirovano et al. / Surface Science Reports 62 (2007) 219–270 on reduced TiO2 surfaces. The ultraviolet photoemission spectroscopy (UPS) spectra of single-crystal surfaces contain a band gap feature at ∼1 eV below the conduction band edge, which has been interpreted in terms of occupied Ti 3d states [131,132], a view supported by the resonant behavior of UPS across the range of photon energies corresponding to the Ti 3p–3d excitation threshold [133–136].
Moreover, UPS measurements on preparation induced reduced rutile (110) surface (e.g., annealing or Ar bombardment) showed a band gap state at 0.7–0.9 eV below the conduction band [137,138] for low defect concentration that moves towards the bottom of the conduction band as the defect concentration increases [139, 140]. This is consistent with EELS studies ; the signature of surface oxygen vacancies is a loss feature at about 0.9 eV. Furthermore, a shoulder in the Ti 2p spectra seen in X-ray photoelectron spectroscopy (XPS) was attributed to TiIII ions, and the lack of surface conductivity also evidence the localized nature of the additional electrons .
3.3. Reduced TiO2 rutile (110) surface There are two possible types of states that the electrons left in TiO2 systems (bulk and surface) upon reduction can occupy: delocalized conduction band states (its bottom formed by Ti 3d states) which leads to a metallic ground state, or localized Ti 3d states in the band gap connected with an insulating ground state. The latter type corresponds to the experimental observations. TiIV ions in titania are in the d0 state, TiIII ions formed upon oxygen removal are in the d1 state. The excess charge localization seriously challenges DFT calculations as anticipated in Section 2, and shown next and in Section 3.5.
3.3.1. Structure relaxation and electronic structure Studies of reduced TiO2 surfaces using Hartree–Fock or hybrid DFT methods, where the Fock exchange is partially mixed with the DFT exchange, are relatively scarce [8, 12,23,25]. Mackrodt et al.  performed spin-unrestricted Hartree–Fock (UHF) calculations  of the fully reduced (1 × 1)TiO2(110) surface (Θdef = 1) that included relaxation of the surface structure upon reduction. The surface model contained three layers (all were allowed to relax). The term layer is used for the repeating O–Ti2O2–O unit (see Fig. 2). For other computational details see Table 1.
The largest displacements were those of the oxygen atoms in the outermost Ti–O plane, which moved outwards by up to ∼0.3 Å. The UHF calculations led to an antiferromagnetic insulating, ground state, i.e., an open-shell singlet. The excess-electron density was located solely at the surface and evenly distributed between the nearest and next-nearest neighbors to the defect. The occupied states associated with the Ti(4) (Ti(6) before defect formation, cf. Fig. 1) and Ti(5) atoms were entirely separated from each other. (Note that the fourfold coordination results of the fact that Θdef = 1). They were located in the band gap within ∼1–2 eV of the top of the valence band.
Bredow and Pacchioni  modelled the isolated defect limit for the TiO2(110) surface using cluster models, and discussed the defect formation energy (see Section 3.3.2). Clusters of different size were either embedded in point charges (Ti4O8 and Ti10O20) or terminated by hydrogen atoms [Ti4O8 (H2O)8, Ti10O20 (H2O)12, Ti17O34 (H2O)19]. The oxygen defect was created by removing the central bridging oxygen atom from the surface. The spin-polarized unrestricted (UKS) calculations were performed using two hybrid functionals with 20% and 100% Fock exchange, B3LYP and HFLYP, respectively (Table 1).
The structures of the reduced clusters were only partially reoptimized. Removal of one oxygen atom did not result in an open- shell singlet ground state, but in a triplet state (Table 1). For the largest (unrelaxed) system the energy difference between the triplet and closed-shell singlet state was 0.39 eV. The two unpaired electrons were almost equally distributed over the two fivefold (Ti(6) in the defect free surface) nearest neighbors to the defect, and the two next-nearest neighbors (Ti(5)), before structure relaxation was considered. However, after relaxation the excess electrons localized almost entirely on the two Ti(5) next-nearest neighbors, probably to reduce electron repulsion.
With the HFLYP functional this localization was present even in the unrelaxed structures. Thus, localization is in part connected with the defect-induced structural relaxations. Beyond that, the difference between the B3LYP and HFLYP results confirms the awaited “sensitivity” of the results to the main approximations made.
Zhang et al.  considered a fully reduced 5L slab (Θdef = 1.0) and applied the hybrid density functional proposed by Moreira et al.  with an admixture of 13% of Fock exchange into spin-polarized LDA. The (empirical) value of 13% was determined by fitting the calculated value of the bulk band gap as a function of the percentage contribution of Fock exchange to the experimental value (3.0 eV). The B3LYP functional (20% exchange) overestimated the band gap by ∼0.5 eV. The ground state was a triplet, but the antiferromagnetic solution (open- shell singlet) was only 13 meV less stable. For 13% Fock exchange within LDA, two defect states ∼2.4 eV above the top of the valence band were predicted, i.e., approximately 0.6 eV below the conduction band edge (cf.
Table 1). The resulting spin density is mainly localized on the Ti(4) (Ti(6) before reduction) and Ti(5) surface atoms, with major dx2−y2 (Ti(4)) and dxz (Ti(5)) contributions, however small density contributions are still seen on cations belonging to the layers beneath (see Fig. 3). Recently, Di Valentin et al.  performed spin-polarized calculations using the B3LYP functional for a 4L c(2 × 4) reduced slab (Θdef = 1/4). The structure was fully relaxed, except for the atoms in the bottom layer which were fixed at their bulk positions. We note that in the (a0 × b0) nomenclature of the (reduced) surface unit cells two choices are possible, namely the a0- and b0-axis parallel to the bulk [1̄10] and  directions, respectively, or viceversa.
Within the former choice the (1 × 1) surface unit cell has dimensions of √ 2a × c with a and c the bulk lattice parameters (aexp = 4.59 Å and cexp = 2.95 Å) . In the following, we will use this choice as the standard nomenclature and indicate differences (if any) with the original literature.
The c(2 × 4) structure allows for the possibility of having inequivalent nearest and next-nearest neighbors to the defect.
M.V. Ganduglia-Pirovano et al. / Surface Science Reports 62 (2007) 219–270 225 Table 1 Bridging oxygen defect on TiO2(110) as obtained by different methods (see Section 3.3.1) Methoda Core-electrons Basis set Modelb Θdef Spin state Electronic structurec References HF All-electron Ti:86-411(d3)G; O:8-411G 3L slab 1 Open-shell singlet Two occupied defect states ∼1–2 eV above O 2p band in the gap; excess electrons localization on all surface Ti atoms Mackrodt et al.
 B3LYP Ti: ECPd Ti: [8s5p5d/ 3s3p(2d)]; O: 6-31G Cluster Isolated Triplet Excess electrons localization on two Ti next-nearest neighbors Bredow and Pacchioni  Hybrid 13% Focke All-electron Ti:86-411(d3)G; O:8-411G 5L 1 Triplet Two occupied defect states at ∼2.4 eV above O 2p band in the gap; excess electrons localization mainly on all surface Ti atoms Zhang et al.  B3LYP All-electron Ti:86-411(d41)G; O:8-411(d1)G 4L 1/4 Triplet Two occupied defect states at 1.1 and 0.9 eV below the conduction band in the gap; the excess electrons remain on one nearest and one next-neareast Ti neighbor Di Valentin et al.
 Non-spin LDA US PP 340 eV 3L 1/2, 1 Non-spin Metallic ground state; excess electrons localization mainly at Ti surface atoms Ramamoorthy et al.  PW91 Kleinman– Bylander 750 eV 3L 1/2, 1 Triplet Insulating ground states; occupied defect states above O 2p band in the gap (e.g., ∼0.7–1.8 eV, Θdef = 1); localization solely at Ti surface atoms (Θdef = 1) and at Ti surface and subsurface atoms (Θdef = 1/2) Lindan et al.  LDA/PW91 All-electron LMTO 3L 1 Triplet Metallic ground state; local magnetic moments 1.2 (Ti under bridging O), 0.6 (fivefold), and 0.2µB (subsurface) Paxton and Thiên-Nga  PW91 US-PP 396 eV 3L 1/3, 1/2 Triplet Not discussed Menetrey et al.
 PW91 US-PP 396 eV 3L–5L 1/2, 1 Triplet Electron density gain upon reduction fairly delocalized over the slab Vijay et al.  PW91 US-PP 396 eV 3L–7L 1/2, 1/4 Triplet Not discussed Oviedo et al.  PBE US-PP 340 eV 4L 1/6, 1/4, 1/2 Triplet Excess electrons localization primarily at Ti atoms near to the defect Wu et al.  PW91 US-PP 340 eV 3L–6L 1/6, 1/4, 1/3, 1/2 Triplet Defect states right below conduction band edge; spread of the excess electrons (after relaxation) with a sizable amount accumulating at the near Ti atoms Rasmussen et al.  a Spin-polarized (unrestricted Kohn–Sham) calculations except otherwise noted; the low spin solution was assumed closed-shell if not mentioned otherwise in the original work.
b L (layer) is used for the repeating O–Ti2O2–O unit.
c In all studies electrons left in the system occupied Ti 3d states. d Ti core: 1s2 to 2p6; O: all-electron. e Hybrid functional , 13% Fock-exchange, 87% LDA.
226 M.V. Ganduglia-Pirovano et al. / Surface Science Reports 62 (2007) 219–270 (a) Top view. (b) Side view. Fig. 3. Distribution of the spin density calculated by hybrid LDA+13% Fock for the reduced TiO2(110) (1×1) surfaces. The dashed lines in (a) indicate the surface unit cell, and the distribution on the outermost three layers. Note that the unit cell axis differ from the standard nomenclature.
Figure reproduced with permission from Zhang et al. . c 2005, American Chemical Society. Fig. 4. Spin up-projected density of states of the c(2 × 4) reduced TiO2(110) surface, calculated using the B3LYP functional. Blue and yellow spheres indicate titanium and oxygen ions, respectively. The vertical dotted line in the plot denotes the position of the Fermi energy. Figure reproduced with permission from Di Valentin et al. .
c 2006, by the American Physical Society. The results show that rather than localizing on the two next- nearest neighbors (Ti(5)) as predicted by Bredow and Pacchioni , one electron localizes on a nearest neighbor and the other on a next-nearest neighbor. The reason why the B3LYP cluster and periodic calculations differ may be the limited relaxation considered in the cluster, which signalizes the importance of accounting for full geometry optimization. Fig. 4 shows the spin up-projected total density of states. The states at 1.1 and 0.9 eV below the bottom of the conduction band correspond to the occupied Ti 3d states localized on one Ti(5) and one of the the former Ti(6) atoms, respectively.
The studies reported so far employed cluster or supercell approaches and used exact exchange or a portion of it (cf. Table 1). The same physical picture emerges from all of them: The excess electrons occupy (strictly) localized Ti 3d states. The hybrid methods predicted location of these states below the conduction band edge (0.6–1.1 eV) is in fairly good agreement with experimental results (0.7–0.9 eV, cf. Section 3.2). What remains experimentally unresolved is the existence of two distinct states.
The LDA and gradient-corrected approximation have been widely and frequently used [7,9–11,13–18,22,28].
The first (non-spin-polarized) self-consistent LDA calculation  of reduced TiO2(110) surfaces was performed by Ramamoorthy et al.  They used supercells containing three (3L) and five layer (5L) slabs (for other computational details see Table 1). The attention was focused on the 3L (1 × 2) and (2 × 1) supercells, for which only one half of the bridging oxygen atoms were absent (Θdef = 1/2), as well as on the fully reduced (1 × 1) structure (Θdef = 1). The (2 × 1) configuration has alternate  oriented rows of bridging oxygen defects, whereas the (1 × 2) has alternate oxygen defects along each such row.
The two unit cells differ with respect to the closest distance between defects. For the (1×2) cell this equals 2·c and is twice as large as for the (2 × 1) cell. Ramamoorthy et al.  found the (1×2) structure to be lower in energy by 0.13 eV (3L slab).
Geometry relaxation upon reduction was considered, however, it is likely that only the atoms in the outermost (slab) layer were allowed to move. The resulting (1×1) geometry was very close to that found in Ref. , despite those calculations were performed using the UHF approach. In the relaxed (1 × 2) structure, both surface Ti atoms that were bonded to the removed bridging oxygen were displaced by 0.1 Å away from the defect along the  direction. Note that for lower defect concentrations than Θdef = 1, the structure relaxations obtained with the LDA or GGA functionals may vary from those obtained with approaches that use exact exchange, in cases in
M.V. Ganduglia-Pirovano et al. / Surface Science Reports 62 (2007) 219–270 227 which the localization of the excess electrons as described by the different functionals differ . The electrons left at the (110) reduced surfaces (Θdef = 1/2, 1) occupy Ti 3d states localized primarily on all surface Ti atoms. These states were found not to be separated by a gap from the bottom of the conduction band in gross disagreement with experiment. Lindan et al. [9,10] considered the same systems as Ramamoorthy et al. , but performed spin-polarized PW91 calculations. The defect induced surface relaxations were in broad agreement with those of Ref.
 (largest displacement of ∼0.4 Å for the oxygen atoms in the outermost Ti–O plane), but the (2 × 1) structure was found to be more stable than the (1 × 2) structure by ∼0.2 eV. This corresponds to a difference in surface energy of 0.04 J/m2, which the authors indicated to be at the limit of accuracy of their calculations. Lindan et al.  found a triplet ground state for all structures investigated (cf. Table 1). Large energy differences between the (closed-shell) singlet and triplet solutions were reported (e.g., ∼3 eV for the (2 × 1) cell). In the following, we assume that the authors did not search for an open-shell singlet solution if they did not mention this explicitly.
For the (1 × 1) structure, each surface Ti atom received one electron upon reduction. Fig. 5 shows the corresponding spin-projected total density of states. A band at 0.7–1.8 eV above the top of valence band corresponds to the Ti 3d occupied states. The lowest unoccupied states (not shown) are about 1.9 eV above the valence band edge of the defect free system. Thus, the occupied states are in the gap. Although optical properties and band gaps are not ground-state properties, it has become a common practice to compare DFT one electron energies with experimentally measured quasi-particle spectra.
It is well- known that the LDA usually underestimates band gaps for semiconductors and insulators [145,146]. For TiO2 (rutile) the predicted LDA band gap is around 2.0 eV [147–149], (exp.: 3.0 eV). Using gradient-corrected functionals such as PW91 does not necessarily improve the results , and the HF approximation yields a band gap that is three times larger than the experimental one . Therefore, we expect that the actual position of defect states within the gap may not be accurately predicted using any of these methods. The deviation between the B3LYP and the experimental band gaps is less severe, as previously mentioned.
For the (2 × 1) configuration the associated occupied Ti 3d states lay 0.2–0.8 eV above the top of valence band in the gap, whereas for the (1 × 2) configuration they were higher in energy (0.8–1.5 eV). The spin density distributions showed that no electron localizes on surface Ti atoms that would be fivefold coordinated at the defect-free surface but on one nearest Ti neighbor to the defect (Ti(6) before reduction), and one Ti atom in the middle layer. We note that Lindan et al.  indicated the possibility that these reduced systems have multiple minima on the potential energy surface determined by the starting geometry.
Namely, once one electron is localized on a Ti ion in the course of structure optimization, subsequent structural relaxation may not be enough to allow the electron to move to another site.
Fig. 5. Spin-projected density of states of the (1×1) reduced TiO2(110) surface within the PW91 approximation. The zero of the energy scale has been set at the highest occupied energy state. The lowest unoccupied states (not shown) are located at about +0.1 eV. Figure reproduced with permission from Lindan et al. . c 1997, by the American Physical Society. The existence of gap states is in agreement with the findings using hybrid DFT methods and spin-polarized Hartree–Fock [8,12,23,25], and in contrast to those (spin-paired) of Ramamoorthy et al.  obtained with plain DFT (cf. Table 1).
This comparison may suggest that including spin-polarization is necessary and sufficient to reproduce the observed n-type semiconducting character of the ground state of reduced TiO2 systems (cf. Section 3.2). This qualitative agreement between the hybrid and GGA approaches should not be assumed to exist always. Nevertheless, it is surprising that non-spin-polarized calculations of oxygen defects at the TiO2(110) surface are still being published .
Paxton and Thiên-Nga  applied the spin-polarized all- electron full-potential linear muffin-tin orbital (FP-LMTO) [152,153] method to a 3L slab model of the fully reduced (1×1) TiO2(110) surface. Exchange and correlation was treated within both the LDA [154,155] and PW91 approximations. Both bulk truncated and relaxed atom positions (those reported in Ref. ) were considered. In no case an occupied state in the band gap was found (cf. Table 1). The Ti local magnetic moments were 1.2µB and 0.6µB (LDA) for the Ti surface atoms that were sixfold and fivefold coordinated, respectively, at the defect free surface and 0.2µB on Ti atoms of the central layer.
Thus, the excess electrons were, as a result, to some extent delocalized. The all-electron spin-polarized calculation by Paxton and Thiên-Nga  is at odds with that by Lindan et al. , however, results obtained using all-electron and pseudopotentials methods (and the same functional) are expected to be (at least) qualitative similar. If not, one should worry about the quality of the pseudopotential used (see later discussion in this section).
A great amount of work [13–19] on reduced TiO2(110) over recent years, using periodic boundary conditions and ultra-soft pseudopotentials, has led to an understanding of the above- stated disagreements and to an answer to the question: What is the electronic structure of reduced TiO2 in the context of DFT- GGA methods? With the recent increase in computational resources, thicker (up to 7L) slabs and lower defect concentrations (up to
228 M.V. Ganduglia-Pirovano et al. / Surface Science Reports 62 (2007) 219–270 Table 2 Selected atomic displacements (in Å) (relative to the positions of the relaxed defect-free surface) upon formation of an oxygen defect in (1 × 4) cell  Atoma ∆y ∆z O(1) −0.027 0.007 O(2) 0.043 0.006 O(3) −0.008 0.122 Ti(4) −0.225 −0.296 Ti(5) 0.209 −0.298 O(6) −0.006 0.274 Ti(7) −0.023 −0.186 Ti(8) 0.020 0.187 ∆x = 0 for all atoms.
a The labels in parenthesis correspond to those in Fig. 6. Θ = 1/6) have been investigated. The importance of considering thicker systems will become apparent later. Among all periodic studies on reduced TiO2(110) using gradient- corrected functionals and (ultra-soft) pseudopotentials, the one by Rasmussen et al.  is probably the most systematic (and most accurate). They performed spin-polarized PW91 calculations and investigated defect concentrations in the range 1/6 < Θdef < 1/2 using slabs of varying thickness (3L–6L) and (1 × 6), (1 × 4), (1 × 3), and (1 × 2), and c(2 × 6), c(2 × 4), and c(2 × 2) unit cells.
The centered cells correspond to Θdef = 1/6, 1/4 and 1/2, respectively. At a given concentration, with respect to the distance between defects along the  direction (i.e., in the rows) both the primitive and centered cells are identical. However, in the centered cells the periodicity is doubled in the [1̄10] direction (i.e., a0) and the two oxygen rows are displaced by b0 with respect to each other. (In the original work the orientation of the a0 and b0 lattice vectors is interchanged.) The use of both primitive and centered cells of increasing size allowed for an estimation of defect interactions along and across the bridging rows (see Section 3.3.2).
Geometry relaxations (beyond the first layer) were considered in detail.
Table 2 reproduces the main atomic displacements for the example of the (1 × 4) structure calculated with a four layer slab of which two were relaxed (cf. Fig. 6). The Ti atoms just below the missing O are strongly pushed sideways and down, whereas the O atom below these two Ti atoms are lifted upwards considerably, and relaxations in the second layer are non-negligible. The amplitude of the displacement of the oxygen atoms in the outermost Ti–O plane is not as large as previously reported for 3L deficient slabs at Θdef = 1/2 and 1 [7,10]. The importance of atomic relaxations for reduced rutile TiO2(110) is also apparent in the electronic structure as already mentioned in connection with the results of Bredow and Pacchioni  and further discussed next in this section.
Nevertheless, information of the atomic structure was not in general provided or was considered in restrictive ways. Menetrey et al. , Vijay et al. , and Oviedo et al.  performed spin-polarized PW91 calculations [156,157], as Rasmussen et al.  (cf. Table 1). The former employed (1 × 3) and (1 × 2) unit cells and a 3L slab for which motions were restricted to the outermost layer. They also reported that removal of bridging oxygen atoms causes substantial changes Fig. 6. Illustration of the structural rearrangements upon single defect formation in a (1 × 4) cell (Θdef = 1/4) obtained with PW91.
Figure reproduced with permission from Rasmussen et al. .
c 2004, American Institute of Physics. in the positions of the remaining atoms, leading to an increase of the Ti–Ti distance between nearest Ti neighbors to the defect by 0.41 and 0.28 Å for Θdef = 1/3 and 1/2, respectively, in particular. Vijay et al.  used a (1 × 2) unit cell and considered both Θdef = 1/2 and 1 with 3–5 layer slabs, whereas Oviedo et al.  employed up to 7L slabs and (1 × 2), (2 × 1), and (1 × 4) cells (Θdef = 1/2 and 1/4, respectively). Vijay et al.  fixed only the atoms in the bottom layer in their bulk positions, i.e., the number of layers allowed to relax varied with slab thickness.
Nevertheless, they only described the movements of the atoms in the outermost layer, which agree with those discussed previously [7,10,13]. Oviedo et al.  did not fix any atom in the slabs, but did not report the resulting geometries. Similarly, Wu et al. , who performed spin-polarized calculations [158,159] with the PBE functional using (2 × 3), (1 × 4) and (2 × 2), and (1 × 2) unit cells, where all atoms (except those in the bottom slab layer) were allowed to relax, did not describe the atomic displacements. In these four most recent GGA studies [15–18] the ground states of all oxygen deficient structures considered were triplet (cf.
Table 1), in agreement with most of the earlier investigations [9,11–13]. The (spin-paired) singlet state was found to be less favored by a few tenths of an eV (or less) [16,17]. Such difference qualitatively agrees with that obtained in hybrid periodic  (∼0.01 eV with respect to the open- shell singlet) and cluster  studies (∼0.4 eV), but it is in disagreement with that reported by Lindan et al.  (about 3
M.V. Ganduglia-Pirovano et al. / Surface Science Reports 62 (2007) 219–270 229 eV). Moreover, the late GGA calculations that employed (ultra- soft) pseudopotentials, showed a metallic ground state [15,17, 18] (cf. Table 1). The absence of Ti 3d occupied states in the gap is in agreement with the earlier all-electron calculation of Paxton and Thiên-Nga , but in contrast to the results of Lindan et al. , who used norm-conserving pseudopotentials. It is comforting to see that all-electron and pseudopotential GGA studies do give the same answer. Ref.  includes a hint that there may be some problem with the pseudopotential used by Lindan et al.
. Nevertheless, while the agreement between recent GGA studies is satisfying, they do not reproduce the experimentally observed state in the band gap. Such a state is consistent with the occupation of localized Ti 3d states, whereas in the metallic state electrons are obviously delocalized. The extent to which the excess electrons were found to spread over the system differed considerably [15,17,18]. For example, Vijay et al.  evaluated the electron density loss upon binding of one O atom to reduced (unrelaxed) structures as a qualitative measure of the (de)localization of the excess electrons upon reduction.
Thereby assuming that the electron density loss (when the defect is “healed”) and gain (when the defect is created) are likely to be similar. They calculated the electron density difference ∆ρ = ρfree − ρdef − ρO; ρfree and ρdef are the electron densities of the clean and (unrelaxed) reduced surfaces, respectively, and ρO that of a free O atom at the defect’s position. ∆ρ is negative in those regions where oxygen bonding induces a depletion of electron density. Fig. 7 shows the result for the example of Θdef = 1/2 with (1 × 2) periodicity. The region that is depleted is fairly delocalized over the slab.
Therefore, the delocalization of the excess electrons over many Ti atoms (i.e., not just those connected to the bridging oxygen) was pointed out. Rasmussen et al.  evaluated the actual changes in charge density upon defect creation and found that structural rearrangements are strongly coupled with important changes in the electronic structure as illustrated next for the example of the defect structure at Θdef = 1/4. Fig. 8(a) shows the induced charge density changes upon reduction for the (1 × 4) structure with unrelaxed atoms positions (i.e., equal to those in the relaxed clean TiO2(110) surface).
The excess electrons remained relatively near the defect site mostly at the two closest surface Ti atoms. However, when atoms were allowed to relax (cf. Fig. 8(b)), the excess electrons spread out. The delocalization of the excess electrons increased upon relaxation, however, a sizable amount remained at the nearby Ti atoms. Note the different scales in Fig. 8(a) and (b). Wu et al.  also found the two electrons primarily on those Ti atoms. Consistently with these findings, the calculated density of states of the reduced systems shows a defect related occupied state right below the Fermi level, however, not separated by a gap from the conduction band as already mentioned.
From the above survey we conclude that the answer to the question on the existence of occupied Ti 3d states in the band gap and the corresponding localization of the excess electrons, depends strongly on the exchange–correlation functional used (cf. Table 1). Periodic spin-polarized GGA approaches failed to reproduce the splitting of the occupied Ti 3d states from Fig. 7. Electron density loss when defects at the (1 × 2) reduced TiO2(110) surface (3L slab) are healed as obtained with PW91. The contour corresponds to ∆ρ = −0.040 electrons/Å3. Arrows indicate the positions of the former defect Ti nearest neighbors.
Note that the unit cell nomenclature is different from that used in Ref. . Figure reproduced with permission from Vijay et al. .
c 2002, American Institute of Physics. the bottom of the conduction band. In contrast, HF, B3LYP, HFLYP, and LDA (13% Fock admixture) calculations, which make use of exact exchange, provided the expected localization independent of the model (cluster or periodic) employed. The use of different approximations to exchange and correlation lead not only to considerable disagreements in the calculated electronic structure but also to important quantitative differences in the energy for the removal of lattice oxygen as discussed next.
3.3.2. The rutile TiO2(110) surface defect formation energy Among the hybrid DFT studies on the reduced TiO2(110) surface, only in that by Bredow and Pacchioni  was the energy to form an isolated oxygen defect discussed.
They used the oxygen atom as reference (i.e., EO f in Eq. (1)). The defect formation energy depends strongly on the cluster model used. It was lower when the clusters were embedded in point charges (4.79–4.90 eV, unrelaxed geometries) than for the case of H- termination (from 6.75 to 7.27 eV, also unrelaxed). For the larger Ti17O34 (H2O)19 cluster used EO f is 7.27 eV. If referred to 1 2 O2 (Eq. (2), with E 1 2 O2 d = 5.20 eV in B3LYP ), the defect formation energy becomes E 1 2 O2 f = 4.67 eV. Lattice relaxations will lower these values (cf. Table 3). A decrease of 1.95 eV as calculated for the smaller Ti10O20 (H2O)12 cluster (obtained in a restricted open-shell calculation), leads to an estimate of E 1 2 O2 f ≈ 2.7 eV for the isolated defect with the B3LYP functional (cf.
Menetrey et al. , who considered a (thin) 3L slab (allowing only the outermost layer to relax), obtained EO f =